0 downloads
0 Views
2MB Size

Letter pubs.acs.org/NanoLett

Local and Nonlocal Fraunhofer-like Pattern from an Edge-Stepped Topological Surface Josephson Current Distribution Jae Hyeong Lee, Gil-Ho Lee, Joonbum Park, Janghee Lee, Seung-Geol Nam, Yun-Sok Shin, Jun Sung Kim, and Hu-Jong Lee* Department of Physics, Pohang University of Science and Technology, Pohang 790-784, Republic of Korea S Supporting Information *

ABSTRACT: We report a surface-dominant Josephson eﬀect in superconductor− topological insulator−superconductor (S−TI−S) devices, where a Bi1.5Sb0.5Te1.7Se1.3 (BSTS) crystal ﬂake was adopted as an intervening TI between Al superconducting electrodes. We observed a Fraunhofer-type critical current modulation in a perpendicular magnetic ﬁeld in an Al−TI−Al junction for both local and nonlocal current biasing. Fraunhofer-type modulation of the diﬀerential resistance was also observed in a neighboring Au−TI−Au normal junction when it was nonlocally biased by the Al−TI−Al junction. In all cases, the Fraunhofer-like signal was highly robust to the magnetic ﬁeld up to the critical ﬁeld of the Al electrodes, corresponding to the edge-stepped nonuniform supercurrent density arising from the top and rough side surfaces of the BSTS ﬂake, which strongly suggests that the Josephson coupling in a TI is established through the surface conducting channels that are topologically protected. KEYWORDS: Topological insulators, Josephson coupling Fraunhofer interference pattern, surface pair current

S

coupling via the side surfaces of a TI, which depended most critically on the topological protection. In our study, the side surfaces of a TI were also in contact with the S electrodes, which led to a highly persistent Fraunhofer-like pattern, with respect to increasing the magnetic ﬁeld perpendicular to the top and bottom surfaces. The persistent character of the Fraunhofer-like modulations, corresponding to a Josephson current distribution that was uniform along the top surface and nonuniformly edge-stepped in the Al−TI−Al junction, indicated the existence of the Josephson current on the rough side surfaces as well as the top surface of the TI ﬂake between two Al electrodes. This conﬁrms that the Josephson coupling was conﬁned in all the surface conducting channels, which have topologically protected robust characters. We also obtained Fraunhofer-like diﬀraction modulations of Josephson critical current across the Al−TI− Al junction and diﬀerential resistance across the Au−TI−Au junction in a nonlocal measurement conﬁguration, where the bias current and potential were measured between the diﬀerent sets of junctions. This “mirage” Fraunhofer signal in the nonlocal conﬁgurations provided additional conﬁrmation of the robust surface Josephson coupling. We ﬁrst explain the scheme of monitoring the surface conduction separated from the bulk conduction in terms of the current ﬂow in a hypothetical device shown in Figure 1. We assume that the device consists of a normal (N) conductor and

trong spin−orbit (SO) interaction of carriers in combination with time-reversal symmetry leads to a new quantum state of matter known as topologically insulating electronic phases.1−12 A three-dimensional (3D) topological insulator (TI) is characterized by the presence of an insulating state with an inverted band gap in its bulk and a topologically protected ungapped Dirac-band state on its surface. On a TI surface, the spin polarization of a carrier is tightly linked to its momentum direction13 and the Majorana Fermionic state14 is predicted to be excited at the interface of an s-wave-superconductor−TI hybrid structure.15,16 Superconductor−topological insulator−superconductor (S− TI−S)-type Josephson coupling has recently been experimentally conﬁrmed, based on Bi2Se3,17−20 Bi2Te3,21,22 strained HgTe,23 and BixSb2−xSe3,24 with a dissipationless supercurrent, which is revealed as the superconducting order of the two closely separated S electrodes spatially overlaps across the intervening TI layer. An S−TI hybrid structure is a key element for searching for the Majorana Fermionic state and realizing topologically robust conductive devices. Thus, it is essential to conﬁrm the proximity coupling via the surface channels of a TI, which is separated from the bulk channels, as a step toward inducing a superconducting state in an S−TI hybrid structure. In previous studies of the Josephson eﬀect in TIs, superconducting electrodes were often arranged on the top surface of a TI. The magnetic ﬁeld modulation of the junction critical current (Fraunhofer diﬀraction pattern) exhibited features corresponding to a uniform Josephson current distribution along the width of a junction. In this case, the Fraunhofer pattern did not include the information on the Josephson © 2014 American Chemical Society

Received: April 29, 2014 Revised: July 20, 2014 Published: August 1, 2014 5029

dx.doi.org/10.1021/nl501481b | Nano Lett. 2014, 14, 5029−5034

Nano Letters

Letter

Figure 2. (a) A scanning electron micrograph of the device and the measurement setup used in this study, which consisted of Au electrodes (yellow) and Al electrodes (blue), overlaid on a BSTS ﬂake. IA1B1 (IC1D1) and VA2B2 (VC2D2) are the bias current and voltage diﬀerence between a pair of the Al (Au) electrodes, respectively. x and y denote the spatial coordinates viewed from above. (b) Current− voltage characteristics of the Al−BSTS−Al junction at the bath temperature of 10 mK, where the blue/red curve and arrow denote the sweeping direction of IA1B1 from left/right to right/left. IcA1B1 and IrA1B1 denote the critical and retrapping currents, respectively. (c) The diﬀerential resistance dVA2B2/dIA1B1 of the Al−BSTS−Al junction, obtained by numerically diﬀerentiating the IA1B1−VA2B2 characteristics at diﬀerent values of perpendicular magnetic ﬁeld B, as a function of B and IA1B1 normalized by IcA1B1(0).

Figure 1. A false-colored schematic diagram of devices with nonlocal measurement conﬁgurations, where the electrodes A and B are used as a source and a drain, respectively, for the bias current IAB and the voltage diﬀerence VCD are monitored between electrodes C and D. The normal conductor of the device consists of (a) conducting bulk, (b,c) insulating bulk, and conducting surface. The conducting surface in (c) is superconducting between the electrodes A and B. The arrows denote the current directions in the normal conductors. The crosssection between x1 and x2 corresponds to the dotted x1 −x2 line in Figure 2a.

four electrodes labeled A, B, C, and D shown with crosssectional view, along with the probable current proﬁle via the surface and the bulk. The cross-section is drawn through the middle of the N conductor along the x-axis, which corresponds to the dotted x1−x2 line in Figure 2a. Electrodes A and B are used as the source and drain, respectively, for biasing current IAB, and the potential diﬀerence VCD is monitored between the electrodes C and D. Figure 1a depicts the case in which the N layer is normal-conducting with ﬁnite bulk conductivity. In Figure 1b, the N material consists of an insulating bulk and a conducting surface layer that uniformly covers the entire bulk. This mimics the conduction in a TI ﬂake with normal-metallic contact leads. The situation of Figure 1c is identical to that of Figure 1b with the exception that the electrodes A and B are replaced by superconductors. In Figure 1a, with the electrodes C and D widely separated (>1 μm) from the electrodes A and B VCD is expected to be negligible as the diﬀusive current ﬂow is conﬁned primarily between A and B. In Figure 1b, IAB injected from A spreads out across the entire surface, that is, top, bottom, and four sides, which results in a nonvanishing value of VCD.25 If the electrodes A and B are superconducting and arranged suﬃciently close to one other as in Figure 1c, Josephson coupling is established through the surface conducting layer between electrodes A and B. For IAB less than the superconducting critical current IcAB, the entire current IAB injected from A is conﬁned only between A and B, showing vanishing VCD. For IAB > IcAB, however, the surface conduction between A and B becomes resistive so that IAB injected from A spreads out across the entire surface before being recovered at the drain B, as depicted in Figure 1b, and induces a nonvanishing value of VCD. Thus, in this case, VCD versus B reveals a replica of IcAB versus B, which conﬁrms that

the Josephson coupling occurs dominantly via the surfaceconducting layer. One would not expect this nonlocal mirage Fraunhofer eﬀect for the case of N, sandwiched between the two S electrodes A and B with ﬁnite bulk conduction because in this case the current IAB (>IcAB) would mostly be conﬁned between A and B as in Figure 1a. Only when the conductance in a TI is predominated by the surface conducting layer,25 the situation depicted in Figure 1c is expected. A scanning electron micrograph of the actual device and its measurement conﬁguration is shown in Figure 2a. The setup consisted of a 115 nm-thick BSTS crystal ﬂake, overlaid with Al and Au electrodes. The BSTS ﬂake, grown using the self-ﬂux method,26,27 was mechanically exfoliated onto a Si substrate capped with a 300 nm thick SiO2 layer. Details of the BSTS crystal growing are described elsewhere.28 The Au electrodes were deposited on the BSTS ﬂake by combining electron(e)beam patterning, sequential e-gun evaporation of a Ti/Au (5 nm/350 nm thick and 400 nm wide) bilayer, and lift-oﬀ. Immediately prior to the Ti/Au deposition, the surface of the BSTS ﬂake was Ar ion-beam cleaned for 20 s with a beam power of 4 W (= 400 V × 10 mA). The superconducting Al electrodes were prepared in a similar fashion as the Au electrodes, using a Ti/Al (5 nm/350 nm thick and 400 nm wide) bilayer in place of the Ti/Au bilayer. The thin Ti layers were added to create a good ohmic contact at the BSTS/Al and BSTS/Au interfaces. The electrical leads A1 and B1 (C1 and D1) were the source and drain for current biasing the Al−BSTS−Al (Au-BSTS-Au) junction by IA1B1 (IC1D1), while the potential diﬀerence VA2B2 (VC2D2) across the junction was measured using 5030

dx.doi.org/10.1021/nl501481b | Nano Lett. 2014, 14, 5029−5034

Nano Letters

Letter

ﬂake. Here, the eﬀective penetration depth of the Al electrodes λ was estimated to be about 210 nm, from the relation Φ0 = (L1 + 2λ)WΔB. W(= 5.3 μm) is the width of the junction and Φ0 = h/2e is the magnetic ﬂux quantum. This value of λ agreed with the value in our previous report with Al−graphene−Al Josephson junctions.32 In Figure 2c, the modulation of the junction supercurrent is not reduced rapidly with B but persists over many ﬁeld periods of the envelope modulation almost up to the superconducting critical ﬁeld of the Al electrodes, Bc (≈ 130 G). Notably, IcA1B1 at the ninth lobe in the Fraunhofer-type oscillations is strongly suppressed, the cause of which is not well understood. The diﬀerential resistance dVA2B2/dIA1B1 of the Al−BSTS−Al junction, obtained alternatively by the lock-in technique is shown in Supporting Information 3. The data, having much lower ﬂuctuations, show the behavior very similar to those obtained by dc measurements in Figure 2c, but with smeared boundary of the critical current. It resulted as ΔIcA1B1(B) [ IcA1B1(B) − IrA1B1(B)] reached a value less than

the leads A2 and B2 (C2 and D2), which were equipotential with the leads A1 and B1 (C1 and D1), respectively. The nonlocal potential diﬀerence VD2C2 (VB2A2) was also measured to probe the spatial distribution of IA1B1 (IC1D1) via the surface-conducting channels of the BSTS ﬂake. Josephson coupling was established across the Al−BSTS−Al junction (between the leads A1 and B1), with a spacing of L1 ∼ 190 nm, at temperatures below the critical temperature of Al electrodes. However, with a spacing of ∼1700 nm between the leads B1 and C1, the proximity eﬀect at the Al−BSTS−Al junction did not induce Josephson coupling at the Au−BSTS−Au junction between the leads C1 and D1 with a spacing of ∼1500 nm. Electrical transport properties of the device were examined by measuring dc (I−V characteristics) or ac (diﬀerential resistance) values at bath temperatures between 10 mK and 300 K. The ac measurements were carried out using the conventional lock-in technique at a frequency of 13.3 Hz and a bias current of 10 nA root-mean-square (rms). Figure 2b shows the current−voltage (IA1B1−VA2B2) characteristics of the Al− BSTS−Al junction at a bath temperature of 10 mK, where the arrows indicate the sweeping directions of the bias current IA1B1. At temperatures signiﬁcantly below the critical temperature Tc (= 750 mK) of the Al electrodes, penetration of the superconducting order into the BSTS surface conducting layer was manifested by the presence of a clear supercurrent branch for IA1B1 up to IcA1B1 (≃ 110 nA) in Figure 2b, above which an abrupt switching occurred to a ﬁnite voltage corresponding to the normal-state resistance of approximately 80 Ω. The superconducting phase coherence length ξ was estimated to be 150 nm using the relation of (RN − RS)/RN ∼ ξ/LB1C1. Here, LB1C1 (= 1.7 μm) is the spacing between centers of B1 and C1 and RN (RS) is the resistance of LB1C1 in the normal (superconducting) state of Al electrodes. The hysteretic reverse switching from the resistive to supercurrent state occurred at IrA1B1 (

the lock-in modulation current iA1B1 (= 10 nA) (see Supporting Information 3).

Figure 3. Fits of the observed junction critical current IcA1B1(B), denoted by symbols, to Fraunhofer diﬀraction relation. Black symbols were extracted from the boundary of the pattern in Figure 2c. Critical currents with highly smeared boundary in Figure 2c, which are denoted by orange symbols, were determined by ﬁtting the corresponding IA1B1−VA2B2 curves to Ambegaokar-Halperin model. Red and green curves are best ﬁts using Josephson junction models with edge-stepped nonuniform and uniform supercurrent distributions, respectively. Upper panel of the inset: schematic cross-sectional view of superconducting Al electrodes overlaid on a BSTS ﬂake. Lower panel of the inset: distribution of the supercurrent density JcA1B1 along the y axis. s1 and s2 are the thicknesses of the side and top layers of the BSTS surface, respectively. t (= 115 nm) and W (= 5300 nm) are the thickness and the width of the BSTS ﬂake, respectively. Here, it is assumed that the bottom (light green) of the BSTS surface is in the normal state, the top and two sides of the BSTS surface (cyan) are superconducting, and the BSTS bulk (dark green) is insulating.

Figure 3 shows the normalized critical current IcA1B1(B)/ as a function of B. Black symbols denote the reduced critical current, which were obtained from the boundary of the Fraunhofer pattern in Figure 2c, corresponding to a local maximum of a dVA2B2/dIA1B1 curve. Critical currents with highly smeared boundary in Figure 2c, which are denoted by orange symbols, were determined by ﬁtting the corresponding IA1B1− IcA1B1(0)

5031

dx.doi.org/10.1021/nl501481b | Nano Lett. 2014, 14, 5029−5034

Nano Letters

Letter

in Figure 3, Φ0 was set to be 6.42 G (5.95 G) for the red (green) curve. With the Al electrodes taking on a superconducting state for T < Tc, all of the conducting surfaces of the BSTS ﬂake that were sandwiched between the two Al electrodes in the Al− BSTS−Al junction; that is, the top and two side surfaces of the BSTS ﬂake, became superconducting as a result of proximity coupling, while the bulk and the bottom surface remained insulating and normal-conducting, respectively (see the upper panel of the inset). This produced an edge-stepped nonuniform supercurrent density JA1B1 along the x-direction, as schematically shown in the lower panel of the inset. The magnetic ﬂux dependence of IcA1B1 for the Josephson junction model with the edge-stepped JA1B1(y) is given as35 (see Supporting Information 4)

VA2B2 curves to Ambegaokar−Halperin model.33 The green (red) curve is the best ﬁt to a Josephson-junction model of the Fraunhofer-type magnetic ﬁeld dependence of the maximum Josephson current with uniform (edge-stepped nonuniform) supercurrent density distribution, where the variation of the critical current in proportion to34 the B-ﬁeld-dependent superconducting gap, Δ(B)/Δ(0) = [1 − (B/Bc)2]1/2, is taken into account. A model of the nonuniform supercurrent density provides a far better ﬁt to the observed data than that of a uniform supercurrent density. The equation IcA1B1(Φ/Φ0) = IcA1B1(0)[1 − (Φ/Φc)2)]1/2|[sin(πΦ/Φ0)]/(πΦ/Φ0)| was used to calculate the ﬁt of the uniform supercurrent density,35 where Φ is the magnetic ﬂux threading the Al−BSTS−Al junction and Φc is the value corresponding to the critical ﬁeld Bc. For the ﬁts

( )≃

I Ac 1B1

Φ Φ0

I Ac 1B1(0)

⎛ Φ ⎞2 1−⎜ ⎟ ⎝ Φc ⎠

( st )( Ws − 2) ( st )( Ws − 2) + 2 2

1

⎡ ⎤ ( ) + 2⎛⎜ t ⎞⎟⎛ s ⎞ sin⎢⎣( )( )⎥⎦ cos⎡⎢⎛1 − s ⎞ π Φ ⎤⎥ ( ) ⎝ s ⎠⎝ W ⎠ ( )( ) ⎣⎝ W ⎠ Φ ⎦

sin ×

2

1

πΦ Φ0

πΦ Φ0

Here, s1 and s2 are the thickness of the side and top layers of the BSTS surface, respectively, and t is the thickness of the BSTS ﬂake. In eq 1, for s1, s2 ≪ W as in this study, the B-ﬁeld dependence of IcA1B1 for an edge-stepped current distribution is mainly governed by the factor (t/s2) × (s1/W). For the ﬁxed values of t and W, it implies that the overall shape of the Fraunhofer pattern mainly depends on the ratio of s1/s2. Because of the factor (1 − s1/W) in the second cosinusoidal term, however, the detailed behavior of eq 1 in the high-B-ﬁeld region close to Bc is sensitive to the value of s1 (or, equivalently s2 for a ﬁxed ratio of s1/s2) in comparison with W as well (see Supporting Information Figures S5−S7). The ﬁt of eq 1 to the observed IcA1B1(Φ/Φ0) in Figure 3 is obtained for s1 = s2 ≃ 5.5 and s2 = 1 nm. The quality of the ﬁt is retained as long as s2 < 5 nm but noticeable degradation appears for s2 ∼ 7 nm or beyond as B approaches Bc. This upper-limit value of 5 nm for s2 is in good agreement with the previous report of 6 nm.36 The diﬀerence between s1 and s2 in our device may have resulted from the enhanced roughness25 of the side surfaces of the BSTS ﬂake (see Supporting Information Figure S4). Because of the geometrical factor 2(t/s2)(s1/W) (≃ 1/4) in eq 1, the ﬁrst sinusoidal term predominates for small Φ/Φ0 (∼1), giving rise to the typical Fraunhofer-type variation of IcA1B1. However, as the value of Φ/Φ0 increases suﬃciently beyond 1, the second cosinusoidal term predominates, which represents the typical | cos(πΦ/Φ0)|-type B-ﬁeld modulation of the junction critical current similar to that of a superconducting quantum interference device (SQUID). The second term produces highly persistent ﬁeld-modulation amplitude of IcA1B1 for B up to Bc as seen in Figure 3. It is easy to deduce that the uniform supercurrent distribution inside the edge (inset of Figure 3) corresponds to the Fraunhofer-diﬀraction-type IAc 1B1 ﬁeld modulation while the enhanced edge-stepped nonuniform supercurrent density corresponds to the SQUID-like behavior in eq 1. The B-ﬁeld modulation of the extracted junction critical current shown in Figure 3 agrees well with eq 1, both in its

⎜

2

1

⎟

s1 W

s1 W

πΦ Φ0

πΦ Φ0

⎜

1

⎟

0

(1)

magnitude and ﬁeld periodicity. In fact, the period of ﬁeld modulation of the observed IcA1B1 in Figure 3 in the low ﬁeld range is slightly smaller than that in the high ﬁeld range, which agrees reasonably well with the combined variation with B of the ﬁrst and second terms in eq 1. By contrast, the observed ﬁeld modulation of IcA1B1 is not in phase with the ordinary Fraunhofer behavior with a ﬁxed ﬁeld periodicity for a uniform current distribution (see Supporting Information 5 for more discussion). The good ﬁt of both the magnitude and the periodicity of IcA1B1 to eq 1 up to Bc strongly indicates the edgestepped nonuniform current distribution. This provides clear conﬁrmation of a supercurrent through topologically robust conducting channels of the BSTS TI surface, including the side surfaces. The existence of the topologically protected conducting surface of the BSTS ﬂake was also evidenced by the nonlocal measurements corresponding to the illustrations in Figures 1b and 1c. Figure 4a shows vD2C2 as a function of IA1B1 and B, which is the rms modulation voltage corresponding to iA1B1,D1C1. Here, iA1B1,D1C1 is the fraction of the modulation current iA1B1 (=10 nA) ﬂowing between D1 and C1, when iA1B1 is applied between A1 and B1 in combination with the dc bias current IA1B1. Figure 4a mimics Figure 2c as vD2C2 is sensitive to changes in the spatial distribution of IA1B1 via the BSTS TI surface. vD2C2 vanished for a supercurrent ﬂow (IA1B1 < IcA1B1) through the Al−BSTS−Al junction. For IA1B1 > IcA1B1, however, vD2C2 gave a ﬁnite value corresponding to iA1B1,D1C1 × RD2C2, where iA1B1,D1C1 is a fraction of the modulation current iA1B1 ﬂowing between D1 and C1, and RD2C2 (= 660 Ω) is the resistance across the region. We obtained the result iA1B1,D1C1 = 0.003 × iA1B1 (see Supporting Information 6). The reverse process was also valid with the relation iC1D1,B1A1 = 0.023 × iC1D1, where iC1D1,B1A1 is the fraction of iC1D1 (= 100 nA) ﬂowing between B1 and A1 (see Supporting Information 6). vB2A2 was also sensitive to change in the 5032

dx.doi.org/10.1021/nl501481b | Nano Lett. 2014, 14, 5029−5034

Nano Letters

Letter

superconducting proximity eﬀect between Pb and Bi2Te3 established along the thickness direction of the Bi2Te3 ﬂake. These observations were interpreted in terms of a widely extended proximity eﬀect, including the bulk of the ﬂakes.22 Becasue the bulk transport can be substantial in these materials, this interpretation is plausible. However, considering that the extremely extended Josephson coupling in these reports is not well understood, the nonlocal eﬀect we report here may have been involved in the observation. In summary, we demonstrated a surface-dominant Josephson eﬀect in S−TI−S junctions. This constitutes a direct and unequivocal conﬁrmation of the existence of a dominant surface conduction in BSTS TI ﬂakes28 and Josephson coupling conﬁned to the surface conducting channels when the TI ﬂakes are in proximity to superconductors. The magnetic ﬁeld modulations of the supercurrent of the Al−BSTS−Al junction remained up to the superconducting critical ﬁeld of the Al electrodes. A voltage in part of the TI outside the Al−BSTS−Al junction was nonlocally triggered along with modulations of the junction supercurrent. The voltage across the Al−BSTS−Al junction was also modulated by the nonlocal bias current at the Au−BSTS−Au junction. This mirage Fraunhofer eﬀect can be explained only in terms of the existence of robust surface conducting channels, which extend to the sides of the TI. The local and nonlocal Fraunhofer diﬀraction-type modulation of the junction critical current and diﬀerential resistance with persistent ﬁeld modulation of the envelope shows nice ﬁts to the model of a edge-stepped nonuniform supercurrent density on the rough side surfaces of the BSTS ﬂakes. This strongly suggests that the Josephson coupling in a TI is established through the surface conducting channels that are topologically protected. This study provides a unique method for conﬁrming Josephson coupling via the topological surface conducting channels, which in turn provides a solid basis for exploring Majorana Fermionic excitation states by adopting TI/superconductor heterostructures.

Figure 4. (a) Nonlocal modulation voltage vD2C2 corresponding to iA1B1,D1C1 as a function of the bias current IA1B1 applied between A1 and B1, and magnetic ﬁeld B. iA1B1,D1C1 is the fraction of the modulation current iA1B1 (= 10 nA) ﬂowing between D1 and C1. vD2C2 exhibits Fraunhofer-type variations. The blue-colored (red-colored) inside (outside) region of the pattern denotes the pair-conducting (resistive) state of the Al−BSTS−Al junction. (b) Nonlocal modulation voltage vB2A2 corresponding to iC1D1,B1A1 as a function of the bias current IC1D1 applied between C1 and D1, and magnetic ﬁeld B. iC1D1,B1A1 is the fraction of iC1D1 (= 100 nA) ﬂowing between B1 and A1. vB2A2 also exhibits Fraunhofer-type variations. Temperature increase due to Joule heating altered the shape of the primary peak of vB2A2 around B = 0.

distribution of the bias current IC1D1 via the BSTS TI surface. vB2A2 vanished if IC1D1,B1A1 < IcA1B1 (= −IcA1B1). For IC1D1,B1A1 < IcA1B1, vB2A2 became iC1D1,B1A1 × RB2A2 as shown in Figure 4b, where RB2A2 = 80 Ω was the normal-state resistance between B2 and A2. The appearance of this nonlocal feature indicates the existence of a topologically protected conducting surface on our BSTS ﬂake25 with Josephson coupling across it. The primary lobe of vB2A2 in Figure 4b exhibits a typical Fraunhofer-type modulation but diﬀers from that of vD2C2 in Figure 4a; the diﬀerential resistance is highly enhanced along the edge of the critical current. This diﬀerence resulted from the temperature increase due to Joule heating generated by the bias current IC1D1(≃ 43 IB1A1). IcC1D1 ≃ 3 μA in Figure 4b corresponds to IcB1A1 ≃ 70 nA. The Joule heating due to IC1D1 was transferred to the BSTS ﬂake between B2 and A2 with the carrier temperature in the BSTS ﬂake reaching a temperature of ∼115 mK (see Supporting Information 7). The value of IcB1A1 (≃ 70 nA) was suppressed below 110 nA at T = 10 mK (without Joule heating) as the carrier temperature rose to 115 mK due to Joule heating, which led to the condition ΔIcB1A1(0) < iB1A1, so that enhancement of the diﬀerential resistance at the edge of the critical current recurred, as discussed in Supporting Information 3 in association with Supporting Information Figure S3. Fraunhofer modulation has been reported over an extended volume in Bi2Se3 from the Pb−Bi2Se3 interface by the proximity eﬀect.19 The same group has also reported a strong

■

ASSOCIATED CONTENT

S Supporting Information *

Normal-state properties of the BSTS crystalline ﬂake, overdamped characteristics of the Josephson junction, diﬀerential resistance of the Al−BSTS−Al junction by ac measurements, Fraunhofer interference pattern for a nonuniform supercurrent density, ﬁts to the uniform-current Fraunhofer diﬀraction for diﬀerent ﬁeld periodicity, estimation of the nonlocal current, and suppression of Ic due to bias-induced Joule heating. This material is available free of charge via the Internet at http:// pubs.acs.org.

■

AUTHOR INFORMATION

Corresponding Author

*E-mail: [email protected] Notes

The authors declare no competing ﬁnancial interest.

■

ACKNOWLEDGMENTS This work was supported by the National Research Foundation (NRF) through the SRC Center for Topological Matter (Grant 2011-0030046 for H.J.L., Y.S.S., and J.S.K.), the GFR Center for Advanced Soft Electronics (Grant 2011-0031640 for H.J.L.), the Basic Science Research Program (Grant 5033

dx.doi.org/10.1021/nl501481b | Nano Lett. 2014, 14, 5029−5034

Nano Letters

Letter

(23) Oostinga, J.; Maier, L.; Schüffelgen, P.; Knott, D.; Ames, C.; Brüne, C.; Tkachov, G.; Buhmann, H.; Molenkamp, L. Jopsephson Supercurrent through the Topological Surface states of Strained Bulk HgTe. Phys. Rev. X 2013, 3, 021007. (24) Cho, S.; Dellabetta, B.; Yang, A.; Schneeloch, J.; Xu, Z.; Valla, T.; Gu, G.; Gilbert, M.; Mason, N. Symmetry protected Josephson supercurrents in three-dimensional topological insulators. Nat. Commun. 2013, 4, 1689. (25) Lee, J.; Lee, J.; Park, J.; Kim, J.; Lee, H. Evidence of Distributed Robust Surface Current Flow in 3D Topological Insulators. Phys. Rev. X 2014, 4, 011039. (26) Ren, Z.; Taskin, A.; Sasaki, S.; Segawa, K.; Ando, Y. Optimizing Bi2−xSbxTe3−ySey solid solutions to approach the intrinsic topological insulator regime. Phys. Rev. B 2011, 84, 165311. (27) Taskin, A.; Ren, Z.; Sasaki, S.; Segawa, K.; Ando, Y. Observation of Dirac holes and electrons in a topological insulator. Phys. Rev. Lett. 2011, 107, 016801. (28) Lee, J.; Park, J.; Lee, J.; Kim, J.; Lee, H. Gate-tuned differentiation of surface-conducting states in Bi1.5Sb0.5Te1.7Se1.3 topological-insulator thin crystals. Phys. Rev. B 2012, 86, 245321. (29) Tinkham, M. Introduction to Superconductivity, 2nd ed.; McGraw-Hill: Singapore, 1996. (30) Doh, Y.; van Dam, J.; Roest, A.; Bakkers, E.; Kouwenhoven, L.; De Franceschi, S. Tunable supercurrent through semiconductor nanowires. Science 2005, 309, 272−275. (31) Courtois, H.; Meschke, M.; Peltonen, J. T.; Pekola, J. P. Origin of hysteresis in a proximity Josephson junction. Phys. Rev. Lett. 2008, 101, 067002. (32) Choi, J.; Lee, G.; Park, S.; Jeong, D.; Lee, J.; Sim, H.; Doh, Y.; Lee, H. Complete gate control of supercurrent in graphene p−n junctions. Nat. Commun. 2013, 4, 2525. (33) Ambegaokar, V.; Halperin, B. I. Voltage due to thermal noise in the dc Josephson effect. Phys. Rev. Lett. 1969, 22, 1364−1366. (34) Ambegaokar, V.; Baratoff, A. Tunneling between superconductors. Phys. Rev. Lett. 1963, 11, 104. (35) Barone, A.; Paternò, G. Physics and applications of the Josephson eﬀect; John Wiley & Son, Inc.: New York, 1982; pp 69−91. (36) Peng, H.; Lai, K.; Kong, D.; Meister, S.; Chen, Y.; Qi, X.-L.; Zhang, S.-C.; Shen, Z.-X.; Cui, Y. Aharonov-Bohm interference in topological insulator nanoribbons. Nat. Mater. 2010, 9, 225−229.

2012R1A1A2044224 for Y.S.S.), and the Mid-Career Researcher Program (Grant 2012-013838 for J.S.K.).

■

REFERENCES

(1) Kane, C. L.; Mele, E. J. Quantum spin Hall effect in graphene. Phys. Rev. Lett. 2005, 95, 226801. (2) Hansan, M. Z.; Kane, C. L. Colloquium: Topological insulators. Rev. Mod. Phys. 2010, 82, 3045−3067. (3) Kane, C. L.; Mele, E. J. Z2 Topological order and the quantum spin Hall effect. Phys. Rev. Lett. 2005, 95, 146802. (4) Fu, L.; Kane, C. L.; Mele, E. J. Topological insulators in three dimensions. Phys. Rev. Lett. 2007, 98, 106803. (5) Moore, J. E.; Balents, B. Topological invariants of time-reversalinvariants band structures. Phys. Rev. B 2007, 75, 121306. (6) Roy, R. Topological phases and the quantum spin Hall effect in three dimensions. Phys. Rev. B 2009, 79, 195322. (7) Bernevig, B.; Hughes, T. L.; Zhang, S.-C. Quantum spin Hall effect and topological phase transition in HgTe Quantum Wells. Science 2006, 314, 1757−1761. (8) Fu, L.; Kane, C. L. Topological insulators with inversion symmetry. Phys. Rev. B 2007, 76, 045302. (9) König, M.; Wiedmann, S.; Brüne, C.; Roth, A.; Buhmann, H.; Molenkamp, L. W.; Qi, X.-L.; Zhang, S.-C. Quantum spin Hall insulator state in HgTe quantum wells. Science 2007, 318, 766−770. (10) Hsieh, D.; Qian, D.; Wray, L.; Xia, Y.; Hor, Y. S.; Cava, R. J.; Hasan, M. Z. A topological Dirac insulator in a quantum spin Hall phase. Nature 2008, 452, 970−975. (11) Xia, Y.; Qian, D.; Hsieh, D.; Wray, L.; Pal, A.; Lin, H.; Bansil, A.; Grauer, D.; Cava, R. J.; Hasan, M. Z. Observation of a large-gap topological-insulator class with a single Dirac cone on the surface. Nat. Phys. 2009, 5, 398−402. (12) Zhang, H.; Liu, C.-X.; Qi, X.-L.; Dai, X.; Fang, Z.; Zhang, S.-C. Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface. Nat. Phys. 2009, 5, 438−442. (13) Hsieh, D.; Xia, Y.; Qian, D.; Wray, L.; Dil, J. H.; Meier, F.; Osterwalder, J.; Pattley, L.; Checkelsky, J. G.; Ong, N. P.; Fedorov, A. V.; Lin, H.; Bansil, A.; Grauer, D.; Hor, Y. S.; Cava, R. J.; Hasan, M. Z. A tunable topological insulator in the spin helical Dirac transport regime. Nature 2009, 460, 1101−1106. (14) Wilczek, F. Majorana returns. Nat. Phys. 2009, 5, 614−618. (15) Fu, L.; Kane, C. L. Superconducting proximity effect and Majorana fermions at the surface of a topological insulator. Phys. Rev. Lett. 2008, 100, 096407. (16) Beenakker, C. Search for Majorana Fermions in superconductors. Annu. Rev. Cond. Matter Phys. 2013, 4, 113−136. (17) Sacépé, B.; Oostinga, J.; Li, J.; Ubaldni, A.; Couto, N.; Gianini, E.; Morpurgo, A. Gate-tuned normal and superconducting transport at the surface of a topological insulator. Nat. Commun. 2011, 2, 575. (18) Williams, J.; Bestwick, A.; Gallagher, P.; Hong, S.; Cui, Y.; Bleich, A.; Analytis, J.; Fisher, I.; Goldhaber-Gordon, D. Unconventional Josephson effect in hybrid superconductor-topological insulator devices. Phys. Rev. Lett. 2012, 109, 056803. (19) Yang, F.; Qu, F.; Shen, J.; Ding, Y.; Chen, J.; Ji, Z.; Liu, G.; Fan, J.; Yang, C.; Fu, L.; Lu, L. Proximity-effect-induced superconducting phase in the topological insulator Bi2Se3. Phys. Rev. B 2012, 86, 134504. (20) Galletti, L.; Charpentier, S.; Iavarone, M.; Lucignano, P.; Massarotti, D.; Arpaia, R.; Suzuki, Y.; Kadowaki, K.; Bauch, T.; Tagliacozzo, A.; Tafuri, F.; Lombardi, F. Influence of topological edge states on the properties of Al/Bi2Se3/Al hybrid Josephson devices. Phys. Rev. B 2014, 89, 134512. (21) Veldhorst, M.; Snelder, M.; Hoek, M.; Gang, T.; Guduru, V.; Wang, X.; Zeitler, U.; van der wiel, W.; Golubov, A.; Hilgenkamp, H.; Brinkamn, A. Josephson supercurrent through a topological insulator surface state. Nat. Mater. 2012, 11, 417−421. (22) Qu, F.; Yang, F.; Shen, J.; Ding, Y.; Chen, J.; Ji, Z.; Liu, G.; Fan, J.; Jing, X.; Yang, C.; Lu, L. Strong superconducting proximity effect in Pb-Bi2Te3 hybrid structures. Sci. Rep. 2012, 2, 339. 5034

dx.doi.org/10.1021/nl501481b | Nano Lett. 2014, 14, 5029−5034